Modification of gas diffusion layers properties to improve water management
- 881 Downloads
In this paper we report an approach to improve water management of commercial GDLs by introducing hydrophobicity patterns. Specifically, line and grid patterns have been created in the MPL side by laser radiation. For an in-depth investigation of these modified GDLs the current density distribution was monitored during fuel cell operation. Additionally, the physical properties of these materials were investigated by a number of ex situ methods such as Fourier transform infrared microscopy, electrochemical impedance spectroscopy and water vapor sorption. Furthermore, a comparison of the physical properties of the patterned GDLs with chemically modified GDLs (treated in H2SO4 and H2O2) is provided. Our results show a clearly improved homogeneity of current density distribution of the patterned GDLs compared to untreated GDLs. This observation is likely due to a reduced local hydrophobicity which facilitates water diffusion along the flow field of the fuel cell. However, performance of the fuel cell was not affected by the MPL irradiation.
KeywordsFuel cell GDL Water management Performance PTFE Laser patterning
In a polymer electrolyte membrane fuel cell (PEMFC) the gas diffusion layer (GDL) is used for proper distribution of reactants to the catalyst layer and for the water management within the membrane electrode assembly (MEA) making the GDL a key component responsible for appropriate and continuous fuel cell operation [1, 2]. The GDL is typically divided into two parts—the macroscopically porous GDL backing and the microporous layer (MPL) . Both parts are treated with poly(tetrafluoroethylene) (PTFE) to obtain specific hydrophobicity needed for fuel cell operation. Flooding of the active catalyst layer (CL), where the reactions take place  is avoided by transporting the water away from the reaction layer due to the hydrophobic behavior of GDL [5, 6]. Water produced inside the fuel cell can flood the pores of GDL and decrease the gas permeability of the layer promoting fuel starvation [7, 8, 9]. Moreover, excess water can drag the platinum particles from the CL, so that the electrochemical processes efficiency is lowered . On the other hand, a drying out of the membrane has to be avoided to assure adequate ionic conductivity . Furthermore, the MPL provides an effective current collection and a smooth, continuous interface between GDL and CL  reducing the ohmic losses in the fuel cell and enhancing chemical and mechanical stability of the CL and the membrane .
Within this paper we address the possibility of improving GDL properties by locally changing its hydrophobic properties by patterning it via laser radiation, i.e., by locally burning PTFE. The main idea of this modification was the fact that water management can be positively affected by varying the PTFE content in the GDL [11, 13]. In recent studies the non-homogeneous distribution of PTFE was investigated [11, 14, 15]. It was concluded that the appropriate ratio of hydrophobic and hydrophilic regions can improve the water management in a fuel cell .
We have also considered a treatment of the samples with sulfuric acid or hydrogen peroxide to affect the PTFE coating of carbon fibers  leading to a severe loss of hydrophobicity as reported by Borup et al. . Then we have compared laser patterned GDLs with chemically treated samples to evaluate the differences between these two methods of the PTFE content modification.
For chemical modification the GDL samples were exposed to 1 M hydrogen peroxide or 1 M sulfuric acid solutions for 24 h in 80 °C [16, 18]. These modified samples were immersed in deionized (DI) water to remove the residues of solution. After that the samples were dried in a temperature chamber for 2 h at 80 °C.
Fuel cell test conditions
To test the pristine and patterned GDLs in fuel cell operation we used a 5 × 5 cm2 cell with a single serpentine flow field. The cell was operated in galvanostatic mode with H2 and air in co-flow configuration. The cell operation temperature was 80 °C. Above 0.3 A cm−2 the H2 stoichiometry and oxygen stoichiometry was set to 1.5 and 2.0, respectively. The relative humidity (RH) was controlled by the bubbler temperature and was set to 50%. The gas outlet absolute pressure was 1.5 bar.
A DLR home-made segmented board with 7 × 7 segments and 5 × 5 cm2 was used for current density distribution monitoring [19, 20]. The board was installed at the anode side. In Fig. 1 the scheme of the flow field with the indicated segments is plotted.
The segmented board consists of current collector segments placed on the surface of an epoxy-glass resin matrix. For the local current measurement a resistor array is integrated in the printed circuit board. The gas supply is mounted from the back side of the measuring board. The back layer of the board is connected by conducting wires with the front (flow field) which is divided into segmented cells to avoid lateral conduction along the flow field. The current and voltage signals from the segmented board are measured with a multiplexer and a digital multimeter; the data acquisition system of the segmented cell is independent of the control system of the fuel cell test bench. The width of the channel and the land was 1.1 and 0.8 mm, respectively. The inlet is at segment G1, whereas segment A7 is the location of the gas outlet (see Fig. 1).
Ex situ techniques
For local Fourier transform infrared (FTIR) analysis of PTFE in the laser patterned MPL a Bruker Vertex 80v FTIR spectrometer coupled with a Bruker Hyperion 3000 microscope was used. A typical FTIR microscopy image  consists of an array of numerous measuring points each measured in the attenuated total reflection (ATR) mode using a conical Ge crystal (diameter of the tip is 100 μm) that is pressed onto the sample for good mechanical contact, i.e., high signal to noise ratio. For high lateral resolution (1 μm) each measuring position (32 × 32 μm2) was detected with a liquid nitrogen cooled mercury–cadmium–telluride focal plane array (FPA) detector consisting of 64 × 64 pixels. Typical spectra were recorded with 2 × 2 binning (32 × 32 superpixels) in the range of 600–4000 cm−1 with 4 cm−1 resolution and consist of typically 32 accumulated scans.
For detailed investigation of surface structure and morphology, the samples were scanned with a Jeol JCM-5000 electron microscope.
The electrical properties were studied with electrochemical impedance spectroscopy (EIS) using a Solartron 1287A/1260 facility. This method can be used to determine the dependency of electrical impedance on frequency of the applied electrical field. To ensure a proper contact between the sample and the electrode a special sample holder was developed and liquid electrodes (mercury) were used.
Through-plane conductivity of pristine, chemically modified and irradiated GDLs was studied in frequency range from 0.1 Hz to 20 MHz at ambient conditions. Excitation amplitude was set to 10 mV.
The thermal stability of the samples was investigated in the temperature range from 25 to 1000 °C with a thermogravimetry analyzer (MTGA, Q500) in a nitrogen atmosphere; the heating rate and the nitrogen flow were set to 10 °C min−1 and 40 ml min−1, respectively. During the temperature increase, it is possible to detect the thermal decomposition of materials and the content of inert residues. Thermal stability measurements of GDLs provide information which can be relevant for MEA preparation processes such as hot pressing .
The absorption and desorption processes related to water uptake were studied with dynamic gravimetric water sorption analyzer (DVS ET, Surface Measurement Systems). During this measurement the mass of the sample is monitored and the humidity in the measuring cell is dynamically regulated. The difference in absorption and desorption processes is represented by sorption isotherm and its hysteresis.
Results and discussion
In this section first the characterization of the laser patterned GDLs by FTIR microscopy and scanning electron microscopy (SEM) is discussed. Secondly, the influence of the laser patterning on fuel cell performance is analyzed based on the local current density distribution. To better understand the behavior of the laser patterned layers the physical properties of these samples are compared with those of chemically modified GDLs.
By means of laser radiation simple patterns of straight lines (pattern 1) and grid (pattern 2) were created on the MPL surface (see Fig. 1). The distance between lines was approximately 2–3 mm and the line thickness was about 0.5 mm. The patterns were created by horizontal motion of the laser beam. The effect of the irradiation on the MPL with a laser beam is basically identical with a highly local heating of the material. This leads to burning, carbonization and/or evaporation of the surface components. It has been observed, that irradiation of the microporous layer media with 350 mW at 532 nm almost instantly burns holes or trenches into the material.
Figure 2b, c show, respectively, the FTIR microscopy image and a corresponding line scan of the MPL side (the signal corresponds to peak areas of the CF2 stretch vibrations in the range 1100–1300 cm−1), which has been locally irradiated (two parallel lines corresponding to the blue color in the spectroscopic image) according to the procedure described above. Evidently within the burned lines the C–F2 vibrational intensity is virtually zero, while it is high outside the lines.
The surface of the irradiated GDLs was scanned with the electron microscope (Fig. 2) whereby two imaging methods were used. In Fig. 2d the imaging mode based on the detection of secondary electrons is used. The burned lines are clearly visible as dark regions. However, the GDL backing is not recognizable: this fact suggests that only a small surface region of the MPL is affected. The same sample was scanned using the method based on backscattered electrons detection (Fig. 2e). This method provides additional information about the GDL surface. Obtained image shows the superficial deterioration of the MPL caused by laser irradiation.
For the performance tests the two patterns were prepared out of an MPL for 25 cm2 single cell and were mounted on the cathode side. The line patterned specimen was mounted in the test cell with the grafted trenches orthogonally to the overall flow field channels; for the grid pattern, the mounting direction was irrelevant. To assembly the MEA a commercial catalyst coated membrane (Johnson Matthey) was used. The cell was equipped with a DLR home-made segmented board to monitor the current density distribution.
However, the cells with the different GDLs exhibit substantial differences regarding current density distributions. In Fig. 4a current density distributions recorded at different loads using pristine and patterned MPLs are shown. In the provided test the humidification of gases was 50% RH. Evidently, in the case of the pristine MPL the maximum current density is located clearly in the gas inlet region. At the cell outlet the performance is worst. The homogeneity of the distribution, represented by the value a (percentage of values that are within ± 20% of average), is around a = 60–80%.
On the other hand, the current density distributions measured with the patterned MPLs show a maximum shifted to the centre of the cell with a significantly improved homogeneity with a = 90–100%.
The improved homogeneity of the current density distribution along the flow field is clearly related to a decreased local hydrophobicity [11, 22]. Thereby, both tested patterns behave similarly suggesting that in the used co-flow configuration only a small change of MPL’s hydrophobicity is sufficient to obtain significantly more homogeneous current density distribution. In this context, it may be stated that a more homogeneous current density distributions would likely extend the life time of the fuel cell, as mentioned in [23, 24]. It should be noted that the water management is influenced by many effects, e.g., water removal due to high reactant flow rate  or GDL oxidation by substances as hydrogen peroxide and sulfuric acid degrades fuel cell operation [16, 26].
The results of thermal stability measurement show significantly faster decomposition of chemically modified GDLs (Fig. 5b) compared to pristine and lasered samples. The steep decrease of sample mass between 500 and 600 °C is related to PTFE decomposition [31, 32]. Rapid mass loss above 600 °C can be caused by structural deterioration of GDL or change of functionalization of the carbon fiber surface (formation of the carboxyl groups). Solutions used for chemical modification may influence the carbon fibers and the diffusion layer becomes less stable during the temperature increase. Diluted solutions can oxidize carbon fibers  and this corrosion process results in formation of substances such as phenol and carboxyl groups .
The samples were also investigated with respect to water vapor sorption and desorption (see Fig. 5c). This measurement can be used for the determination of a volume density of hydrophobic regions. Water vapor is stored in the hydrophilic regions and the increase of the sample mass can be detected. Thereby the amount of sorbed water is represented by the hysteresis. In case of pristine GDL the volume density of hydrophobic regions is larger than in case of chemically modified or irradiated GDLs leading to a narrow hysteresis. Similarly, the sample treated by sulfuric acid shows a small hysteresis suggesting virtually no impact of this treatment on the hydrophobicity. In contrast, hydrogen peroxide affects the PTFE coating leading to a severe volume density loss of the hydrophobic regions and a large hysteresis. A significant increase of sample mass was measured for irradiated samples pointing at their reduced hydrophobicity compared to other samples and supporting FTIR analysis where a loss of hydrophobic PTFE was clearly observed. Since the lasered area is larger in pattern 2 than in pattern 1, its hysteresis is larger accordingly (see Fig. 5c). The possible explanation is that the partly burned MPL strongly affected a water uptake of irradiated GDL and the water diffusion was facilitated [11, 33].
The GDL Sigracet 24BC was irradiated with laser beam and simple patterns of burned lines were created. The thermal, electrical and sorption properties were studied for pristine chemically modified and laser irradiated samples.
The performance test of MEA containing irradiated GDL was conducted and the current density distribution was investigated. Under the operation conditions used, the results show significantly more homogeneous current density distribution when patterned GDLs were used compared to pristine GDLs. This is likely due to an improvement of the water management changing local hydrophobicity leading to a facilitation of water diffusion and removal along the flow field. An influence of the laser irradiation on the performance of the fuel cell was not observed.
For detailed analysis of the physical properties of the patterned GDLs, further GDLs were modified by sulfuric acid and hydrogen peroxide for comparison. Electrical conductivity of chemically modified samples increased with respect to PTFE content decrease. Water sorption of the sample exposed to hydrogen peroxide increased due to the loss of the density of hydrophobic regions (the impact of sulfuric acid was weak). The thermal stability measurement of the chemically modified GDLs showed rapid decrease of sample mass during heating.
The result was developed within the CENTEM project, reg. no. CZ.1.05/2.1.00/03.0088, co-funded by the ERDF as part of the Ministry of Education, Youth and Sports OP RDI programme and, in the follow-up sustainability stage, supported through CENTEM PLUS (LO1402) by financial means from the Ministry of Education, Youth and Sports under the National Sustainability Programme I. The research leading to these results has received funding from the European Union’s Seventh Framework Programme (FP7/2007–2013) for Fuel Cell and Hydrogen Joint Technology Initiative under Grant 303446 (IMPALA).
- 17.Borup, R.L., Meyers, J., Pivovar, B., Kim, Y.S., Mukundan, R., Garland, N., Myers, D., Wilson, M., Garzon, F., Wood, D., Zelenay, P., More, K., Stroh, K., Zawodzinski, T., Boncella, J., McGrath, J.E., Inaba, M., Miytake, K., Hori, M., Ota, K., Ogumi, Z., Miyata, S., Nishikata, A., Siroma, Z., Uchimoto, Y., Yasuda, K., Kimijima, K.-I., Iwashita, N.: Scientific aspects of polymer electrolyte fuel cell durability and degradation. Chem. Rev. 107, 3904–3951 (2007)CrossRefGoogle Scholar
- 22.Pauchet, J., Prat, M., Schott, P., Pulloor, Kuttanikkad S.: Performance loss of proton exchange membrane fuel cell due to hydrophobicity loss in gas diffusion layer: analysis by multiscale approach combining pore network and performance modelling. Int. J. Hydrog. Energy 37, 1628–1641 (2012)CrossRefGoogle Scholar
- 23.Rangel-Hernandez, V.H., Damian-Ascencio, C., Juarez-Robles, D., Galegos-Munoz, A., Zaleta-Aguilar, A., Plascencia-Mora, H.: Entropy generation analysis of a proton exchange membrane fuel cell (PEMFC) with a Fermat spiral as a flow distributor. Heat transfer phenomena and application. Intech, Rijeka (2012). ISBN 978-953-51-0815-3Google Scholar
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.